- About this Journal
- Abstracting and Indexing
- Aims and Scope
- Annual Issues
- Article Processing Charges
- Articles in Press
- Author Guidelines
- Bibliographic Information
- Citations to this Journal
- Contact Information
- Editorial Board
- Editorial Workflow
- Free eTOC Alerts
- Publication Ethics
- Reviewers Acknowledgment
- Submit a Manuscript
- Subscription Information
- Table of Contents
Journal of Nanomaterials
Volume 2012 (2012), Article ID 819403, 6 pages
Preparation and Characterization of Alumina Nanoparticles in Deionized Water Using Laser Ablation Technique
1Applied Nanotechnology Laboratory (ANT Lab), Department of Physics, King Mongkut’s University of Technology Thonburi, Bangkok 10140, Thailand
2Thailand Center of Excellence in Physics, CHE, Ministry of Education, Bangkok 10400, Thailand
Received 9 August 2012; Accepted 23 October 2012
Academic Editor: Jian Wei
Copyright © 2012 Veeradate Piriyawong et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Al2O3 nanoparticles were synthesized using laser ablation of an aluminum (Al) target in deionized water. Nd:YAG laser, emitted the light at a wavelength of 1064 nm, was used as a light source. The laser ablation was carried out at different energies of 1, 3, and 5 J. The structure of ablated Al particles suspended in deionized water was investigated using X-ray diffraction (XRD). The XRD patterns revealed that the ablated Al particles transformed into γ-Al2O3. The morphology of nanoparticles was investigated by field emission scanning electron microscopy (FE-SEM). The FE-SEM images showed that most of the nanoparticles obtained from all the ablated laser energies have spherical shape with a particle size of less than 100 nm. Furthermore, it was observed that the particle size increased with increasing the laser energy. The absorption spectra of Al2O3 nanoparticles suspended in deionized water were recorded at room temperature using UV-visible spectroscopy. The absorption spectra show a strong peak at 210 nmarising from the presence of Al2O3 nanoparticles. The results on absorption spectra are in good agreement with those investigated by XRD which confirmed the formation of Al2O3 nanoparticles during the laser ablation of Al target in deionized water.
Metal oxide nanoparticles have been extensively developed in the past decades. They have been widely used in many applications such as catalysts, sensors, semiconductors, medical science, capacitors, and batteries [1–6]. Among them, aluminum oxide (Al2O3) and its compounds have long been known for more than a century, for example, aluminum oxide hydroxide (AlOOH) and aluminum trihydroxide (Al(OH)3).
Al2O3 or alumina generally refers to corundum. It is a white oxide. Alumina has several phases such as gamma, delta, theta, and alpha. However, the alpha alumina phase is the most thermodynamically stable phase. In general, alumina has many interesting properties, for example high hardness, high stability, high insulation, and transparency . Alumina is also widely used in the fire retard, catalyst, insulator, surface protective coating, and composite materials [8–12].
Al2O3 nanoparticles can be synthesized by many techniques including ball milling, sol-gel, pyrolysis, sputtering, hydrothermal, and laser ablation [13–18]. Among them, the laser ablation is a widely used technique for the synthesis of nanoparticles since it can be synthesized in gas, vacuum or liquid. This technique offers several advantages such as rapid and high purity process compared with other methods . Furthermore, nanoparticles prepared by the laser ablation of materials in liquid are easier to be collected than those of in gas atmosphere.
In the recent years, Al2O3 nanoparticles were synthesized in liquid using a short pulse laser with the pulse width in the range of nanosecond [20–22]. Furthermore, Al target was used as a starting material for laser ablation in those works. Therefore, in this study we reported the synthesis of Al2O3 from Al powders using laser ablation in deionized water with a long pulsed Nd:YAG laser. The laser pulse widths adopted in this work were 2.5, 6, and 9.5 ms to obtain the output laser energies of 1, 3, and 5 J, respectively. The particle size and morphology of synthesized nanoparticles obtained at different laser energies were investigated by field emission scanning electron microscopy (FE-SEM). The optical property of synthesized nanoparticles was carried out using UV-visible spectroscopy. The structure of the synthesized nanoparticles was investigated using X-ray diffraction (XRD) technique.
2. Experimental Setup
2.1. Material Preparation for Laser Ablation
Aluminum powder with purity of 99.99% (American Elements) and an average particle size of 35 μm were pressed in a stainless steel mold by a hydraulic with a pressure of 100 bars to obtain the aluminum pellet with a diameter of 15 mm and 5 mm thick. The aluminum pellet was used as a target for laser ablation. The experimental setup of the laser ablation is shown in Figure 1. The aluminum pellet was placed at the bottom of a glass vessel with a diameter of 30 mm and 50 mm in height. Deionized water with a volume approximately of 10 mL was poured into the vessel until its level was approximately 5 mm above the target. The Nd:YAG (Miyachi, ML-2331B) that emitted the laser light at a wavelength of 1064 nm was used for the laser ablation. The laser ablation was carried out at different laser energies of 1, 3, and 5 J with a repetition rate of 2 Hz. The laser beam was focused by a 50 mm focal-length lens onto the aluminum pellet. For each energy of laser ablation, the aluminum target was ablated with 5,000 pulses for the total time of about 40 min. After the laser ablation, the Al2O3 particles suspended in deionized water was obtained.
After the laser ablation of Al target in deionized water was carried out, the Al particles suspended in deionized water were characterized to confirm that they transformed into Al2O3. The ablated Al particles suspended in deionized water were used for the optical measurement. The optical absorption spectra were recorded at room temperature using a UV-Vis spectrophotometer (JASCO, V570). Then, the liquid sample was dropped on silicon wafers and dried in an oven at 40°C for 4 h. The dried-particles sample on silicon substrates was used for investigating the structure and morphology. The structure of particles was investigated using X-ray diffraction (PANalytical, X’Pert Pro) with CuKα radiation and a pattern recorded at grazing incidence angle (3°) in the 2θ range of 20°–80° with a scan step of 0.02 in a scan time of 5 s. The morphology of particles was investigated using field emission scanning electron microscopy (Hitachi, S4700).
3. Results and Discussion
3.1. The Structure of Ablated Particles
The structure of ablated particles was investigated by XRD measurement. To identify the structural difference between ablated particles and Al, the XRD measurement for Al target was also carried out. Figure 2 shows the XRD patterns of Al target and particles synthesized from laser energies of 1, 3, and 5 J. The observed peaks in Figure 2 could be indexed based on pure Al and γ-Al2O3 phase in Joint Committee on Powder Diffraction Standard-International Center for Diffraction Data (JCPDS-ICDD) Card nos. 85-1327 and 29-0063, respectively. It is seen from the XRD spectra that all particles obtained from laser ablation with different laser energies are γ-Al2O3. This confirms that Al transformed into γ-Al2O3 after the ablation in deionized water. Moreover, it is clearly observed that the intensity of XRD peaks increased with increasing laser energy. This might lead to the conclusion that the particle concentration, suspended in deionized water, obtained from a laser energy of 5 J is higher than those of 1 and 3 J.
It should be pointed out that the phase transitions in aluminum oxide occur in the following order : Since γ-Al2O3 occurs at the lowest temperature compared with those of another phases, the most likely phase of Al2O3 to be formed after laser ablation of Al target in deionized water is γ-Al2O3.
3.2. Morphology of Al2O3 Nanoparticles
The morphology of dried Al2O3 nanoparticle samples obtained from the laser ablation of aluminum pellet in deionized water at different energies was investigated using field emission scanning electron microscopy. For comparison, the morphology of aluminum powder was also investigated. Figure 3(a) shows the FE-SEM image of the aluminum powder used as the target. It revealed that the morphology of the aluminum was a nonspherical shape with the size in the range of 1–35 μm. Figures 3(b)–3(d) show the FE-SEM images of the Al2O3 nanoparticles synthesized in deionized water with different laser energies of 1, 3, and 5 J, respectively. It is clearly observed that the morphology of the synthesized Al2O3 nanoparticles is mostly spherical shape. These results are in good agreement with those previously reported in reference [20–22].
The particle size distribution of the Al2O3 nanoparticles could be obtained by measuring the size of total particles of about 200 particles in the FE-SEM image using the Image J program. The plots of the particle size distribution of the Al2O3 nanoparticles are shown in Figure 4. The average particle size of the Al2O3 nanoparticles is summarized in Table 1. As seen in Figure 4, the particle size of the Al2O3 nanoparticles synthesized in deionized water with laser energies of 1, 3, and 5 J are ranged from 10 to 60, 10 to 70, and 10 to 110 nm, respectively. The average particle size of the Al2O3 nanoparticles as given in Table 1 showed that the smallest particle size of the Al2O3 nanoparticles was obtained from a laser energy of 1 J and found to be 26 nm with the narrow particle size distribution in the range of 10–60 nm. It is seen that the higher laser energy seemed to promote more collisions between the vapour atoms/ions, to coalesce within the ablated plume and eventually to form larger particles.
It should be noted that the spot size of the laser at the target surface is 0.03 mm2. Hence, the laser fluence (J/cm2) can be determined and the results are also given in Table 1.
3.3. Optical Property of Al2O3 Nanoparticle in Deionized Water
Figure 5 shows the opacity of deionized water after the laser ablation of Al with different laser energies. It is clearly observed that the opacity of deionized water increases with increasing laser energy. It can be concluded that the opacity of deionized water is proportional to the number of Al2O3 nanoparticles suspended in deionized water. Hence, the Al2O3 nanoparticles obtained from a laser energy of 5 J are higher than those obtained from 3 and 1 J.
Figure 6 shows the absorption spectra of deionized water with suspended Al2O3 nanoparticles obtained from laser energies of 1, 3, and 5 J. A strong absorption peak at 210 nm is clearly observed which confirms the presence of Al2O3 nanoparticles in deionized water [24, 25] and not those of aluminum [26–28]. As seen in Figure 6, the difference of absorbance is due to the different Al2O3 nanoparticle concentrations suspended in deionized water.
To confirm the dependence of the absorbance on the Al2O3 nanoparticle concentration, all the samples of deionized water with suspended Al2O3 nanoparticles were diluted with deionized water to obtain different water concentrations of C/2, C/4, C/8, and C/16, where C is the initial concentration. All the diluted deionized water samples were used for absorption measurements. Figure 7(a) shows the typical absorption spectra of the deionized water with different Al2O3 nanoparticle concentrations obtained from a laser energy of 5 J. It is seen that the absorbance decreases with decreasing concentration. The plot between Al2O3 nanoparticle concentration and absorbance is shown in Figure 7(b). Figure 7(b) shows that the absorbance depends linearly on the Al2O3 nanoparticle concentration. Similar results were also obtained for laser energies of 1 and 3 J.
We have successfully demonstrated that γ-Al2O3 nanoparticles can be synthesized from Al powder by pulsed laser ablation in deionized water. Al powder was pressed to obtain the Al pellet and used as a target for laser ablation. The advantage of using compressed Al powder is that we can sieve the Al powder to obtain small particle size for starting materials of laser ablation. Therefore, it is easier to obtain Al2O3 nanoparticles compared with those obtained from laser ablation of Al plate. The effect of laser energy on the particle size was investigated. It was found that Al2O3 particle size ablated at a low laser energy was smaller than that obtained from high laser energy. However, high laser energy yielded high Al2O3 concentration than that of low laser energy.
This work had been supported by Thailand Center of Excellent in Physics (ThEP) and King Mongkut’s University of Technology Thonburi under The National Research University Project.
- W. Ueda, M. Sadakane, and H. Ogihara, “Nano-structuring of complex metal oxides for catalytic oxidation,” Catalysis Today, vol. 132, no. 1–4, pp. 2–8, 2008.
- T. Gessner, K. Gottfried, R. Hoffmann et al., “Metal oxide gas sensor for high temperature application,” Microsystem Technologies, vol. 6, no. 5, pp. 169–174, 2000.
- J. H. Kim, E. K. Kim, C. H. Lee, M. S. Song, Y.-H. Kim, and J. Kim, “Electrical properties of metal-oxide semiconductor nano-particle device,” Physica E, vol. 26, no. 1–4, pp. 432–435, 2005.
- P. D. Pria, “Evolution and new application of the alumina ceramics in joint replacement,” European Journal of Orthopaedic Surgery and Traumatology, vol. 17, no. 3, pp. 253–256, 2007.
- H. Farsi and F. Gobal, “Theoretical analysis of the performance of a model supercapacitor consisting of metal oxide nano-particles,” Journal of Solid State Electrochemistry, vol. 11, no. 8, pp. 1085–1092, 2007.
- A. C. Dillon, A. H. Mahan, R. Deshpande, P. A. Parilla, K. M. Jones, and S.-H. Lee, “Metal oxide nano-particles for improved electrochromic and lithium-ion battery technologies,” Thin Solid Films, vol. 516, no. 5, pp. 794–797, 2008.
- L. D. Hart, Alumina Chemicals: Science and Technology Handbook, American Ceramic Society, Columbus, Ohio, USA, 1990.
- A. Laachachi, M. Ferriol, M. Cochez, J.-M. Lopez Cuesta, and D. Ruch, “A comparison of the role of boehmite (AlOOH) and alumina (Al2O3) in the thermal stability and flammability of poly(methyl methacrylate),” Polymer Degradation and Stability, vol. 94, no. 9, pp. 1373–1378, 2009.
- I. Lukić, J. Krstić, D. Jovanović, and D. Skala, “Alumina/silica supported K2CO3 as a catalyst for biodiesel synthesis from sunflower oil,” Bioresource Technology, vol. 100, no. 20, pp. 4690–4696, 2009.
- M. Touzin, D. Goeuriot, C. Guerret-Piécourt, D. Juvé, and H. J. Fitting, “alumina based ceramics for high-voltage insulation,” Vacuum, vol. 81, pp. 762–765, 2007.
- A. Keyvani, M. Saremi, and M. Heydarzadeh Sohi, “Microstructural stability of zirconia-alumina composite coatings during hot corrosion test at 1050°C,” Journal of Alloys and Compounds, vol. 506, no. 1, pp. 103–108, 2010.
- R. Lach, K. Haberko, M. M. Bućko, M. Szumera, and G. Grabowski, “Ceramic matrix composites in the alumina/5-30vol.% YAG system,” Journal of the European Ceramic Society, vol. 31, no. 10, pp. 1889–1895, 2011.
- C. B. Reid, J. S. Forrester, H. J. Goodshaw, E. H. Kisi, and G. J. Suaning, “A study in the mechanical milling of alumina powder,” Ceramics International, vol. 34, no. 6, pp. 1551–1556, 2008.
- F. Mirjalili, M. Hasmaliza, and L. C. Abdullah, “Size-controlled synthesis of nano α-alumina particles through the sol-gel method,” Ceramics International, vol. 36, no. 4, pp. 1253–1257, 2010.
- R. Kavitha and V. Jayaram, “Deposition and characterization of alumina films produced by combustion flame pyrolysis,” Surface and Coatings Technology, vol. 201, no. 6, pp. 2491–2499, 2006.
- D. H. Trinh, M. Ottosson, M. Collin, I. Reineck, L. Hultman, and H. Högberg, “Nanocomposite Al2O3-ZrO2 thin films grown by reactive dual radio-frequency magnetron sputtering,” Thin Solid Films, vol. 516, no. 15, pp. 4977–4982, 2008.
- L. Qu, C. He, Y. Yang, Y. He, and Z. Liu, “Hydrothermal synthesis of alumina nanotubes templated by anionic surfactant,” Materials Letters, vol. 59, no. 29-30, pp. 4034–4037, 2005.
- K. Yatsui, T. Yukawa, C. Grigoriu, M. Hirai, and W. Jiang, “Synthesis of ultrafine γ-Al2O3 powders by pulsed laser ablation,” Journal of Nanoparticle Research, vol. 2, no. 1, pp. 75–83, 2000.
- A. Kruusing, Handbook of Liquids-Assisted Laser Processing, Elsevier, 2008.
- Z. Yan, R. Bao, Y. Huang, and D. B. Chrisey, “Hollow particles formed on laser-induced bubbles by excimer laser ablation of Al in liquid,” Journal of Physical Chemistry C, vol. 114, no. 26, pp. 11370–11374, 2010.
- I. L. Liu, P. Shen, and S. Y. Chen, “H+- and Al2+-codoped Al2O3 nanoparticles with spinel-type related structures by pulsed laser ablation in water,” Journal of Physical Chemistry C, vol. 114, no. 17, pp. 7751–7757, 2010.
- B. Kumar and R. K. Thareja, “Synthesis of nanoparticles in laser ablation of aluminum in liquid,” Journal of Applied Physics, vol. 108, no. 6, Article ID 064906, 2010.
- W. H. Gitzen, Alumina as Ceramic Material, special publication no. 4, American Ceramic Society, 1970.
- H. Chang and Y. C. Chang, “Fabrication of Al2O3 nanofluid by a plasma arc nanoparticles synthesis system,” Journal of Materials Processing Technology, vol. 207, no. 1–3, pp. 193–199, 2008.
- V. S. Kortov, S. V. Nikiforov, I. I. Milman, and E. V. Moiseykin, “Specific features of luminescence of radiation-colored α-Al2O3 single crystals,” Radiation Measurements, vol. 38, no. 4–6, pp. 451–454, 2004.
- E. Stratakis, V. Zorba, M. Barberoglou, C. Fotakis, and G. A. Shafeev, “Femtosecond laser writing of nanostructures on bulk Al via its ablation in air and liquids,” Applied Surface Science, vol. 255, no. 10, pp. 5346–5350, 2009.
- G. Viau, V. Collière, L. M. Lacroix, and G. A. Shafeev, “Internal structure of Al hollow nanoparticles generated by laser ablation in liquid ethanol,” Chemical Physics Letters, vol. 501, no. 4–6, pp. 419–422, 2011.
- E. Stratakis, M. Barberoglou, C. Fotakis, G. Viau, C. Garcia, and G. A. Shafeev, “Generation of al nanoparticles via ablation of bulk al in liquids with short laser pulses,” Optics Express, vol. 17, no. 15, pp. 12650–12659, 2009.